Received date: 11 November 2010; Accepted date: 2 December 2010
Visit for more related articles at Bioceramics Development and Applications
biomaterial; titanium; osteointegration; electrospinning; hydroxyapatite
Various metal and metal alloys such as 316L stainless steel, cobalt-based alloys and titanium alloys are frequently used as an implant material for bone plates, screws and hip joint prosthesis . A typical 316L stainless steel is stronger and cheaper but its corrosion properties along with more susceptibility to infection brings inferiority to titanium based alloys. Cobalt alloys exhibit reasonable biodegradation properties when exposed to human tissues, but not as resistant to corrosion as titanium . In relation to implant materials, titanium and titanium alloys are highly regarded as skeletal biomaterials because of their good biocompatibility and bioinertness . This material allows direct bone-to-implant contact that has also been called as “osseointegration” . Unfortunately, like most metals, Ti exhibits poor bioactive properties [8,11]. The biological tissues typically interact with the outermost atomic layers of an implant, and therefore the surface properties of the implant material play a very important role in immediate reactions on the implant surface after exposure to the tissue and influence the osteoconductivity [5,9,11]. In this respect, titanium with its native bioinert surface, it is difficult to achieve good chemical bonding with bones and form new bones on its surface at the early stage after implantation. Hence, titanium and titanium alloys do not meet all the requirements of the “ideal” biomaterial . So, there is the urgent need of surface modification with bioactive material .
Hydroxyapatites, the most ubiquitous family of bioceramics, are attractive as they can be produced in such a way that they mimic the mineral composition and/or the porous structure of bone; form a direct bond with neighboring bone with their ability to induce mesenchymal cells to differentiate towards osteoblasts [4,12]. The incorporation of Ca or P ions into the surface layer and the validity of these results have been confirmed by several different researchers. Present work reports the surface modification of Ti with HAp particulate nanofiber by using a simple electrospinning method for the first time. Such a surface modification of titania nano-architectures by sol-gel-derived HAp nanofibers is cost-effective, enabling the realization of desired platform topologies on existing nonmodified implant materials.
Commercially pure titanium (CP Ti, Grade 2, Ka-Hee Metal Industry Co., Korea), machined into disks (10×10×2mm3), was used as the substrate. The samples were pickled using a mixture of hydrogen peroxide (H2O2) and sulfuric acid (H2SO4). Calcium glycerol phosphate (Ca-GP), calcium acetate (Ca-Ac) and all the reagents were purchased from Sigma-Aldrich Co., USA. Polyvinyl alcohol (PVA, Mw = 65,000 Daltons) was purchased from Dong Yang Chem. Co., Korea. HOBs cell line CCRL-11372 was purchased from ATCC, USA. For electrospinning [1,2], a homogenous aqueous slurry of Ca-GP and CA with Ca/P ratio 1.67 was treated with 9% (w/w) PVA (aqueous) solution in the ratio of 3:7 by wt. to get a clear sol-gel, and electrospun by applying 15 kV at an electrode distance of 15 cm. The fibers were subjected to calcination at various temperatures ranging from 200 °C to 1400 °C. A titanium disk that was electrospun and not calcined is referred to as Ti-HAp, whereas the disks that were electrospun and calcined at temperatures ranging 200–1400 °C are referred to as Ti- HAp 200, Ti-HAp 400 and so on, accordingly. HOB cells were plated at a seeding density of 105 cells/cm2 on the sample surfaces. Cell viability was investigated 6 days after seeding the cells using a commercially available MTT (Sigma Co., USA).
FT-IR spectra (Figure 1) of sol-gel-derived HAp on Ti disks were calcined at various temperatures. The observed PO43– asymmetric stretching mode of vibration is characterized by a strong complex band in the 1180–1000 cm–1 range and a medium intensity band at about 975 cm–1 due to symmetric stretching-induced vibrations. The crystalline HAp generates characteristic OH bands at about 3400 cm–1 and the small peaks at 1700–1450 cm–1 indicated the existence of a Ca–O phase in the structure.
X-ray spectra (Figure 2) showed that the titanium surface has been transformed into rutile when calcined at and above 800 °C in air. The broad diffraction peak at a lower temperature (200 °C) displays that the sol-gel-derived hydroxyapatite is in an amorphous state. Such HAp was crystallized at a higher temperature and the sizes of the crystals were increased with an increasing calcination temperature. The surface morphologies of pure Ti, Ti- HAp and heat treated Ti-HAp disks were AFM (Figure 3). Further, samples calcined at 800 °C show some rod-type crystals in addition to a majority of hexagonal-type crystal. Also, samples calcined at 800 °C were found to have wellattachment of HAp on the surface of their disks. However, this was easily removed in samples calcined at and above 1200 °C. Also, the bioactive rutile TiO2 is abundantly observed at calcination temperatures at and above 800 °C. The hydrophilicity of Ti-HAp 800 was expected to vary when compared with other samples.
Most of the cells examined were flattened, polygonallyshaped and showed an evidence of spreading, as well as numerous, highly-extended filopodia with apparent inter cellular communication (Figure 4). After 6 days of culture, the HOBs showed a polygonal morphology on titanium surfaces. These results indicate that the HOBs are able to spread faster on Ti-HAp 800 surfaces compared to other samples (controlled Ti and Ti-HAp 600) within 6 days of culture. These cells spreading behavior seems to help the cell anchor itself to the Ti-HAp crystals, particularly those that are rod-shaped. To ascertain the long term cytotoxic effects of Ti and Ti-HAp matrices, osteoblasts were cultured up to 6 days. HOBs without a sample matrix were used as our control. The LDH assay was used to compare the extent of cell membrane disruption in the presence of various samples. Neither Ti nor Ti-HAp matrices induced significance damage to the cell membrane. All the samples exhibited a similar absorbance showing no toxicity with HOB proliferation. However, all the samples (Ti and Ti- HAp) showed slightly lower cell disruption than the control.
This study highlighted the surface modification of Ti disks with sol-gel-derived HAp via electrospinning, resulting in an hierarchal structure.The composite matrix thus obtained is found to have a superior topographical structure to former surface modification efforts in its promotion of HOB proliferation. This finding will add a new dimension to the surface modification of implant materials to create an appropriate environment for growth and differentiation of cells.
This research was supported by the Korean Research Foundation (KRF2007-211-D00032, Korean Government Project NO. 10028211) and Center for Healthcare Technology Development, Chonbuk National University, Jeonju 562-756, Korea.
Make the best use of Scientific Research and information from our 700 + peer reviewed, Open Access Journals